thermally conductive organic dielectrics for power ...· thermally conductive organic dielectrics
Post on 29-Jul-2018
Embed Size (px)
Thermally Conductive Organic Dielectrics for Power Electronics and Electric Motors
A. A. Wereszczak, T. G. Morrissey, R. H. Wiles,* and H. Wang Oak Ridge National Laboratory (ORNL) * National Transportation Research Center (NTRC/ORNL)
2013 Vehicle Technologies Annual Merit Review and Peer Evaluation Meeting Arlington, VA 14 May 2013
Project ID: pm037_wereszczak_2013_o
This presentation does not contain any proprietary, confidential, or otherwise restricted information
Project start: October 2010 Project end: September 2013 Percent complete: 83%
Total project funding DOE 100%
FY11: $250k FY12: $150k FY13: $100k
OVT Advanced Power Electronics and Electric Motor (APEEM) Program ORNL/NTRC
SolEpoxy (Epoxy molding compound, EMC, manufacturer)
Ube (powder manufacturer)
Barriers Addressed Reliability and lifetime of power electronic
devices (PEDs) and motor components degrade rapidly with temperature increase.
PEDs and motor components need improved thermal management to operate at higher temperatures.
New paradigms in cooling would enable achievement of higher power densities without compromise to device reliability.
Targets: DOE VTP* 2020 target: 105C Coolant DOE VTP* 2020 target: 4 kW/liter power
* VTP Multi-Year Program Plan 2011-2015
Develop low-cost, high-performance epoxy molding compounds (EMCs) for automotive (AEV, HEV) power electronics and electric motors.
Reduce volume and improve thermal reliability of power electronics and electric motors via improved or new thermal management strategies.
Develop EMCs that have: Sufficient low cost for automotive applications Sustained dielectric performance High thermal conductivity ( 5 W/mK) No magnetic susceptibility Use non-toxic and inexpensive filler Equivalent potting and injection molding
characteristics to existing EMCs
FY12: Model, design, and fabricate filler-containing-EMC having 10x thermal conductivity increase over monolithic epoxy. Achieved: 3.0 W/mK compared to 0.2 W/mK.
FY13: Fabricate a thermally conductive EMC structure with a Joule-heated, surrogate electronic device, measure its maximum temperature, and compare to the maximum temperature when a conventional EMC is used. 30 Sep 2013 On track.
ORNLs mission Deliver scientific discoveries and technical breakthroughs that will accelerate the development and deployment of solutions in clean energy and global security, and in doing so create economic opportunity for the nation
Optimize filler particle size distribution and volume fraction.
Fabricate EMCs with organic matrices that allow transfer molding and potting.
Demonstrate thermal conductivity () 5 W/mK.
Technical Accomplishments (1 of 8)
Identified approximate filler particle size distribution (PSD) and volume fraction (Vol%)
Developed software to predict thermal diffusivity as a function of PSD and Vol%
Transient thermal model developed using PDS and Vol%
Modeled effect of higher on components
Thermal conductivity of 3 W/mK achieved with MgO-filled EMCs which is 2x higher than state-of-the-art EMCs
Invention disclosure submitted on hybrid-filled EMCs
Overview of Year's Accomplishments:
Energy is the defining challenge of our time Technical Accomplishments (2 of 8)
Software Was Developed to Create 2D Images of PSDs That in Turn Enables Thermal Conductivity Modeling
Particle size distribution (PSD) Volume fraction Percolation limit Effects on thermal conductivity
Measured PSDs (bimodal)
Technical Accomplishments (3 of 8)
Transient Thermal Modeling Enables Estimation of EMC
D = diffusivity = thermal conductivity = density Cp = heat capacity T = thickness t50 = time to reach 50% max temp
Temperature as a function of time
Technical Accomplishments (4 of 8)
Power electronic and electric motor component exteriors have low thermal conductivity
Strive to increase their thermal conductivity and enable additional approaches to thermal management
Improved cooling, performance, and reliability
Capacitor Power Module
Technical Accomplishments (5 of 8)
Motor Component FEA Example: Effect of EMC = 0.5 W/mK = 1.0 W/mK = 3.0 W/mK
= 5.0 W/mK = 10 W/mK = 20 W/mK
Tmax = 186C Tmax = 182C Tmax = 168C
Tmax = 158C Tmax = 144C Tmax = 132C
10% temperature decrease with 3 W/mK for this example
Technical Accomplishments (6 of 8)
Power Module FEA Example: Effect of EMC
= 0.5 W/mK = 1.0 W/mK = 3.0 W/mK
= 5.0 W/mK = 10 W/mK = 20 W/mK
Tmax = 170C Tmax = 160C Tmax = 141C
Tmax = 130C Tmax = 115C Tmax = 101C
17% temperature decrease with 3 W/mK for this example
Technical Accomplishments (7 of 8)
Thermal Conductivity of 3 W/mK Achieved with MgO-EMCs
Technical Accomplishments (8 of 8)
High dielectric strength
High electrical resistance
Good thermal conductivity
properties to SOA SiO2-EMCs
SolEpoxy, Inc. (Olean, NY). An established, renowned EMC manufacturer
Supplier to power electronic and motor component manufacturers
Fabricated this project's MgO-EMCs in FY12
Fabricating this project's hybrid-filled EMC blends in FY13.
Ube (Japan). An establish MgO supplier
DOE EERE Office of Vehicle Technologies APEEM Program, J. Miller, ORNL/NTRC: motor components
Seeking EMC thermal conductivity to 5 W/mK via "hybrid" EMCs, which are a blend of MgO and a second filler with higher thermal conductivity
Continue to collaborate with SolEpoxy and VTP APEEM motor R&D to adapt MgO-EMC compositions to coating of stator components
Fabricate a thermally conductive EMC structure with a Joule-heated, surrogate electronic device, measure its maximum temperature, and compare to the maximum temperature when a conventional EMC is used
Relevance: thermally-conductive EMCs will lower maximum operating temperature of automotive PEs and EMs and improve their reliability
Approach: develop low-cost thermally-conductive MgO-EMCs
Collaborations: a primary and established EMCs manufacturer and VTO APEEM power electronic and electric motor projects
= 3 W/mK achieved inexpensively, and MgO-EMCs are processable, electrically resistive, and magnetically insusceptible. 2x higher than state-of-the-art SiO2-EMCs
Identified a cost-performance compromise must be struck to get to 5 W/mK.
Demonstrate that a hybrid-filled EMC that blends (cheap) MgO with a (more expensive) high filler can produce = 5 W/mK.
Implement MgO-EMCs compositions in electric motor stator coatings for R&D in the VTO APEEM Program.
Slide Number 1Slide Number 2Slide Number 3Slide Number 4ORNLs missionSlide Number 6Energy is the defining challenge of our timeSlide Number 8Slide Number 9Slide Number 10Slide Number 11Slide Number 12Slide Number 13Slide Number 14Slide Number 15Slide Number 16Slide Number 17Slide Number 18Slide Number 19Slide Number 20Slide Number 21